# ELASTIC PLASTIC FRACTURE MECHANICS METHODOLOGY FOR 2013-08-30¢ elastic plastic fracture...

date post

26-Dec-2019Category

## Documents

view

6download

0

Embed Size (px)

### Transcript of ELASTIC PLASTIC FRACTURE MECHANICS METHODOLOGY FOR 2013-08-30¢ elastic plastic fracture...

NASA-CR-194129

,-,4

0 0 _ ,.,,4

I ,-- e_

0_ C

_._0

,_ 00.c •,.J 0 • U

0 I-

_'_ _ 0 _w- C

kAJ ..

OwZ

O" LAJ _ 0

I O0 O_ kAJ _._

O0 _

._ O_ _ 0 _-_

v U_ t_ Z ,.-_

0

ELASTIC PLASTIC FRACTURE MECHANICS

METHODOLOGY FOR SURFACE CRACKS

SECOND SEMIANNUAL REPORT

CONTRACT MSFC CONTROL NO. 91-78

NASA MARSHALL SPACE FLIGHT CENTER

HUNTSVILLE, AL 35812 /

Project Monitor:

Mr. Wayne Gregg

Principal Investigator:

Dr. Hugo A. Ernst

Associate Professor

Researchers:

D. W. Boatwright W. J. Curtin

D. M. Lambert

.

GEORGIA INSTITUTE OF TECHNOLOGY

THE GEORGE W. WOODRUFF SCHOOL OF MECHANICAL

Atlanta, GA 30332-0405 ENGINEERING

August 1993

https://ntrs.nasa.gov/search.jsp?R=19940006257 2020-01-20T21:08:31+00:00Z

INDEX

1.2

i. Introduction

1 1

1 2

1 3

1 4

1 6

1 7

General

Elastic Plastic Fracture Mechanics

The Leak Before Burst (LBB) Criterion

This Report

References

Figures

2. Computer Modelling of Surface Crack Growth

3. Finite Element Investigation of Constraint Parameter

o

,

Efforts to Characterize Three-Dimensional Effects Observable

in Two Dimensional Fracture Specimens

Appendix:

Growth.

Computer Program, Computer Model of Surface Crack

i.I General

I. IDtroduction

1.3

The safety and reliability of structures has always been a

matter of vital concern to the aerospace industry. In this

respect, fracture mechanics (FM) is a specially useful

technology, since it can provide a quantitative description of

the capability of structural parts to tolerate flaws. Initially,

FM concepts covered quasi-linear elastic conditions (LEFM).

Later, these methods were further developed to cover more general

situations. Specifically, there was a need to extend these

concepts to include cases where yielding was not necessarily

contained in very small regions, for the case of new and tougher

materials, higher loads, thinner sections, et cei_era. This led

to the development of the so-called Elastic Plastic Fracture

Mechanics (EPFM) Methodology.

To apply these methods, two pieces of information are

needed: the so-called material/specimen response to deformation,

and the material response to crack extension. The former,

obtained by finite element analysis or experimental calibration,

consists of two expressions connecting the J-integral, load P,

load-point displacement v, and crack length a for the specimen

geometry of interest; the latter consists of a characterization

of the way the material resists crack extension for the type of

load applied: J, or a similar parameter, versus crack extension,

for monotonic load, da/dN versus _K or AJ for cyclic loading,

da/dt versus K, C* or C t for creep crack growth, et cetera. It

1.4

is assumed that within some limitations, these curves are

specimen geometry independent, i.e., the curve obtained from a

small laboratory specimen applies to the structural part under

consideration, as well.

A simple computer program can be developed to combine the

two pieces of information mentioned and assess the structural

reliability of the structural part of interest.

It is very important to devote effort to guarantee that the

curve of material response to crack extension is, in fact,

geometry independent. That is, it is important to understand the

limitations of the parameters and/or approaches 1_sed, identify

clearly their limits of validity, and eventually improve the

characterization of the phenomenon, proposing new parameters and

methods to extend the range of applicability of existing models.

1.2 Elastic Plastic Fracture _AIIj_Z_

Specifically, for the case of EPFM applied to monotonic

load, the mentioned limitations are expressed in ter!tls of the

amount of crack extension to ligament ratio, r, the ratio of

ligament to applied J over the yield strength, m, and the ratio

of logarithmic increase of J to logarithmic decrease in ligament,

To overcome some of these limitations, particularly the one

on r, Ernst [i.i] proposed a modified version of J called JM.

Resistance (R) curves plotted in terms of JM were not subjected

to the same limitations as those using J, and in general, showed

1.5

a better correlation between specimens of different size and

geometry.

More recently, this methodology was further extended:

general formulas were developed for JM and JD for growing cracks,

criteria were proposed to identify the limits of applicability of

both parameters, methods were presented to make use of the

information of experimental points beyond this limit, and several

schemes were proposed to extrapolate small laboratory specimen

resistance curves to large amounts of crack extension, using JM,

JD, or other parameters [1.2].

Although the progress made has been significant, and

understanding has been gained on how to represent the R curve

[1.2-1.6], there are still several very important points that

need to be addressed before the method can be safely applied.

Among the most important ones, the need to extend this whole

methodology to include cases involving three dimensions (3D) must

be mentioned.

Specifically, it is mandatory to know how specimen

thickness, constraint, and the possible dependence of the

fracture mechanism on specimen thickness may affect the fracture

resistance.

Ultimately, this knowledge gained from "2D" planar specimens

should be used to explain and predict the behavior of real life

3D defects found in structures, i.e., surface or embedded cracks,

et cetera.

1.3 The Leak Before Burst (LBB) _V_j_L_

1.6

Pressure vessels containing surface flaws are often required

to comply with the so-called LBB criterion. LBB is understood as

the condition in which an assumed initial flaw will grow through

the wall of a pressure vessel and cause leakage rather than

bursting.

In particular, pressure vessels of interest to NASA have to

comply to MIL-STD-1522A Standard General Requirements for Safe

Design and Operation of Pressurized Missile and Space Systems.

This document requires that: (I) a/2c (crack depth to total

width ratio) needs to be in a range from 0.05 and 0.5, and (2)

LBB will occur if Kic/Oop > 2_B 0-5 with _°op < Oys and _ > I.

The rationale behind this expression is that the initial

semi-elliptical flaw will grow in a self-similar manner, i.e.,

keeping a/2c constant until the crack depth a is exactly equal to

the thickness B, as shown in Figure i.I. At that time, it is

considered that the flaw becomes a through crack with a total

length of 2c, with 2c = (2c/a)oB, where the subscript 'o' stands

for 'initial' Finally, to prevent the crack from running

unstably in the longitudinal direction, i.e., bursting, it is

then required that the toughness Kic be bigger than the applied K

given by Kap p = Oop(Kc)0-5

The weaknesses of this Standard are these: (i) the above

equation only holds for a/2c = 0.5, (2) the flaw shape is

considered to always remain elliptical with constant a/2c, and

(3) the whole analysis is based on LEFM concepts.

].7

On the other hand, for the real materials, thicknesses, and

typical flaws of interest, the situation is markedly different

from the one assumed above, as can be seen in Figure 1.2. The

cracks, clearly, do not grow in an elliptical self-similar

manner, but rather in a very complex shape, with a dimension in

the direction parallel to the surface, longer in the interior

than on the surface. Moreover there is no guarantee that this

dimension can be conservatively estimated by taking the

original(2c/a) o and multiplying by B.

1.4 This Project

The EPFM Methodology has evolved significantly in the last

several years. Nevertheless, some of these concepts need to be

extended further before the whole methodology can be safely

applied to structural parts. Specifically, there is a need to

include the effect of constraint in the characterization of

material resistance to crack growth and also te _xtend these

methods to the case of 3D defects.

As a consequence, this project was started as a 36 month

research program with the general objective of developing an

elastic plastic fracture mechanics methodology to assess the

structural reliability of pressure vessels and other parts of

interest to NASA containing defects.

The project is divided into the following tasks.

Task i. _ and Thickness Effects

1.8

This task includes the study of the problem of

constraint and thickness effects, in different specimen

sizes and geometries in materials of intere

Recommended

*View more*